Journal of Membrane Science 451 (2014) 111–116
Contents lists available at ScienceDirect
Journal of Membrane Science journal homepage: www.elsevier.com/locate/memsci
Permeability of electrospun ﬁber mats under hydraulic ﬂow Looh Tchuin (Simon) Choong a, Zafarullah Khan b, Gregory C. Rutledge a,n a b
Department of Chemical Engineering, Massachusetts Institute of Technology, Cambridge, MA 02139, USA King Fahd University of Petroleum and Minerals, Dhahran, Saudi Arabia
art ic l e i nf o
a b s t r a c t
Article history: Received 18 June 2013 Received in revised form 21 September 2013 Accepted 25 September 2013 Available online 1 October 2013
The hydraulic permeabilities of electrospun ﬁber mats are found to be functions of their compressibility. Hydraulic permeabilities of electrospun mats of bis-phenol A polysulfone (PSU) comprising ﬁbers of different mean diameters, annealed at temperatures at and above the glass transition of the polymer, were measured for feed water pressures ranging from 5 kPa to 140 kPa. The electrospun mats experience a decrease of more than 60% in permeability between 5 kPa and 140 kPa, due to the loss of porosity, attributed to ﬂow-induced compression. This behavior is explained using a simple model based on Darcy's law applied to a compressible, porous medium. Happel's equation is used to model the permeability of the ﬁber mats, and Toll's equation is used to model their compressibility. The permeation model accurately estimates the changes in solidity, and hence the permeability of the electrospun mats, over a range of pressure differentials. & 2013 Elsevier B.V. All rights reserved.
Keywords: Permeability Compression Nanoﬁbers Electrospinning
1. Introduction Electrospun ﬁber mats are promising for many ﬁltration applications like coalescence ﬁltration, depth ﬁltration, etc., because of their high porosity ( 40.9) and small inter-ﬁber distances (typically 0.1–10 μm), which provide high permeabilities and high separation efﬁciencies [1,2]. However, electrospun ﬁber mats are also highly compressible , hence their porosity decreases with increasing pressure. This compressibility of the mat can counter the beneﬁts of high porosity in ﬁltration applications. An understanding of the extent of the reduction in permeance upon compression for electrospun ﬁber mats is vital for evaluating their performance relative to other, commercial ﬁltration membranes under conditions relevant for ﬁltration processes. A typical operating pressure for an ultraﬁltration process is 0.1 MPa . The studies of liquid ﬂow through compressible media are diverse. Biot [5,6] developed a theory for the consolidation of porous soil containing a viscous ﬂuid; Mow et al. [7,8] studied the effects of compressive strain on the ﬂuid permeability of articular cartilage. Zhu et al.  and Kataja et al.  modeled water permeation during wet pressing of paper. Jönsson and Jönsson [11,12] modeled ﬁltration through compressible porous media as the gradual transformation of hydraulic pressure into mechanical stress on the porous solid. The main difference between the systems mentioned above is the structure of the porous network,
which affects the expressions of permeability constant and compressibility. Here, we adopt the approach of Jönsson and Jönsson, combined with expressions for the permeability and compressibility of ﬁbrous materials to describe the ﬂux of water through electrospun mats. The permeability of porous ﬁbrous media has been studied extensively. Equations for permeability constants that account for the drag forces exerted on the liquid by the solid medium have been developed for ﬂow through a 2-D array of cylinders that are aligned parallel [13,14] or perpendicular [13,14,15] to the direction of the ﬂow, as well as through 3-D random arrays of cylinders . Mao and Russell [17,18] included the effect of ﬁber orientation in both 2-D and 3-D arrays. Others have also studied the permeability numerically and developed the permeability equations empirically from experimental data [19,20,21]. Electrospun mats can be approximated as planar ﬁbrous networks. From the review by Jackson and James , analytical permeability models for ﬂow perpendicular to a 2-D array of cylinders developed by Happel  and by Spielman and Goren  ﬁt the experimental data well in the solidity range 0.05–0.3 (where solidity is deﬁned as 1— porosity). Since Happel's model is simple, physically-based and does not involve implicit functions of permeability, Happel's equation is chosen for this work unless indicated otherwise. The compressibility of electrospun mats can be described by a power-law equation that correlates the compressive stress (sm) applied to electrospun mats with the solidity (ϕ) of the mats sm ¼ kEðϕn ϕn0 Þ
Corresponding author. Tel.: þ 1 617 253 0171; fax: þ 1 617 258 5766. E-mail address: [email protected]
0376-7388/$ - see front matter & 2013 Elsevier B.V. All rights reserved. http://dx.doi.org/10.1016/j.memsci.2013.09.051
where k is an empirical constant that accounts for variations in the length, contour, and other characteristics of the ﬁber segments
L.T. (Simon) Choong et al. / Journal of Membrane Science 451 (2014) 111–116
between load-bearing contacts; E is Young's modulus of the ﬁber; ϕ and ϕ0 are the solidity under compression and the initial solidity of the ﬁbrous medium at zero stress, respectively; and n is the exponent, which depends on the nature of the ﬁber network. We have previously validated Eq. (1) experimentally for electrospun ﬁber mats , and studied the effect of thermal annealing on compressibility of electrospun mats. For details of the derivation of Eq. (1), the reader is referred to the original work of Toll . In this work we characterize the change in permeability of electrospun mats, which are highly compressible, under ﬂowinduced compression, and explain this behavior through a simple combination of the foregoing analytical models. The details of the modeling framework are described in the following section.
2. Modeling of permeation In Jönsson and Jönsson , the total pressure (Ptot) associated with ﬂuid ﬂow through a porous medium system is the sum of the hydraulic pressure (Ph) that drives the ﬂuid ﬂow through the porous medium, and the mechanical stress (sm) that deforms the porous medium. The mechanical stress arises from the drag of ﬂuid on the interior surfaces of the medium as the ﬂuid ﬂows through it. The drag also results in the drop of the hydraulic pressure in the direction of the ﬂow . The mechanical stress on the ﬁber mat increases in the ﬂow direction because the force propagates via the ﬁber–ﬁber contacts . Therefore, the last layer of the porous medium in the ﬂow direction experiences the largest compression, as shown qualitatively in Fig. 1. The Ptot is equal to the trans-membrane pressure drop, ΔP. The ﬂux of water (J) through an electrospun mat, which is a ﬁbrous porous medium, can be described by Darcy's law: J¼
K dP h μ dz
where K is the permeability constant, μ is the dynamic viscosity of water, and dPh/dz is the hydraulic pressure gradient through the thickness of the mat. The negative sign is due to the convention used in this work, where z ¼0 at the inlet of the mat. Since the sum of sm and Ph is constant (sm ¼Ptot Ph), we can rewrite Eq. (2) in terms of sm. J¼
K dsm μ dz
where D is the ﬁber diameter. Eq. (1) was used to account for the compression of the electrospun mat. Given the basis weight and pressure drop across the membrane, we make an initial guess for ﬂux (J) and integrate Eqs. (5) and (6) from ϕ ¼ϕ0 and sm ¼0 at z ¼0 to sm ¼ Ptot. From the proﬁle thus obtained for ϕ(z), the error in basis weight can be determined, and the value for ﬂux iterated until the correct basis weight is obtained. dz K ¼ dsm Jμ
dϕ 1 ¼ dsm nkEϕn 1
During an experiment, the ﬂux (J) and the trans-membrane pressure drop (ΔP) were measured, from which the permeance, deﬁned as J/ΔP, was computed and compared to that predicted by the model. To convert permeance to permeability, it is also necessary to know the mat thickness during ﬂow; the mat thickness, and thus permeability K, was obtained by application of the model. It should be noted that both ϕ and K are average values in this case, since the mat deforms nonuniformly in the through-plane direction during testing, as indicated by Fig. 1.
3. Experimental 3.1. Materials Bisphenol-A-polysulfone (PSU), purchased from Sigma Aldrich, is a glassy amorphous solid at room temperature, with a glass transition temperature of 188 1C, as measured by Differential Scanning Calorimetry (DSC, TA Q100). N,N-dimethyl formamide (DMF) was obtained from Sigma-Aldrich and used as received, as solvent for preparing the PSU solutions for electrospinning. Formic acid (FA) was added to some solutions in small amounts to modify their electrical properties, to allow some control of ﬁber diameter. Cellulose acetate microﬁltration (MF) membrane with a nominal pore size of 3 μm and thickness of (16772) μm (measured using Agilent UTM as described in Section 3.5) was purchased from Millipore (SSWP02500) and used as received.
The permeability constant for a highly porous ﬁbrous medium has been derived analytically for ﬂow around a cylinder by Happel  ! D2 ϕ2 1 K¼ ln ϕ þ 2 ð4Þ 32ϕ ϕ þ1
t=t Ph + m= Ptot = P Direction of flow Ph = P,
3.2. Fabrication A vertically aligned, parallel plate setup was used for electrospinning, as described elsewhere . The top plate was 15 cm in diameter and charged with a high voltage supply (Gamma High Voltage Research, ES40P) to a voltage in the range of 10–30 kV. The grounded bottom plate, which also served as the collector for the ﬁber mat, was a 15 cm 15 cm stainless steel platform. The tip-tocollector distance was varied from 25 to 35 cm by adjusting the height of the bottom plate. The polymeric solution was loaded into a syringe attached by Teﬂon tubing to a stainless steel capillary (1.6 mm OD, 1.0 mm ID) that protruded 21 mm through the center of the top plate. A digitally controlled syringe pump (Harvard Apparatus, PHD 2000) was used to control the ﬂow rate of the polymer solution in the range of 0.005–0.02 mL/min. 3.3. Post-processing
z Ph = 0,
Fig. 1. Schematic of deformation of an electrospun mat under pressure driven ﬂow. The density of the dots represents qualitatively the degree of compaction (solidity) .
The as-spun mats were annealed thermally in a furnace (Thermolyne Industrial Benchtop Furnace, FD1545M) to strengthen the electrospun mat, as previously reported . The mats were held in plane during the annealing process by draping over a petri dish that is 10 cm in diameter. The PSU mats were annealed at
L.T. (Simon) Choong et al. / Journal of Membrane Science 451 (2014) 111–116
temperatures between 190 and 210 1C, which are above the glass transition temperature (Tg ¼188 1C) of PSU, for 1 h. 3.4. Characterization The average ﬁber diameter of the electrospun ﬁber mats was calculated from the measurement of 30–50 ﬁbers in images taken with a scanning electron microscope (SEM, JEOL-JSM-6060). The initial solidity was calculated by ϕ t 0:5 N ϕ0 ¼ 0:5 N ; t0
where ϕ0.5 N is the solidity calculated using a gravimetric method in which the mat thickness (t0.5 N) was measured using an adjustable measuring force digital micrometer (Mutitoyo, Model CLM 1.6″ QM) with a contact force of 0.5 N. The quantity t0 is an estimate of the mat thickness based on the probe position of the Agilent T150 UTM at 20 μN contact force (cf. Section 3.5). 3.5. Compression test An unconﬁned uniaxial compression test was carried out using the Agilent T150 UTM (Agilent Technologies, Chandler, AZ) with a load cell of 500 mN. The electrospun ﬁber mats tend to be metastably hydrophobic due to their texture and porosity. To improve wettability, the mats were plasma treated by a plasma cleaner (Harrick PDC-32G) for 1 min at the low power setting, and then soaked by water right after the treatment. Moreover, the compression test is performed on a wetted sample because the ﬂow-induced compression of the mats occurs in a water-ﬁlled state. Five 1 mm diameter discs were cut from each of the wet, annealed mats using a micro punch with a 1.0 mm tip (TedPella, Harris Micro Punch). Superﬁcial water was removed by capillary action, gently touching the sample surface with a lab tissue to remove the excess liquid. Failure to remove this superﬁcial water led to poor reproducibility of compression results. Each of the discs was subjected to ﬁve cycles of loading and unloading in compression, with a maximum load of 50 mN in each cycle. The ﬁrst four cycles were used to condition the mats, as described previously , and the unloading curve of the ﬁfth cycle was used for analysis. The compression was carried out at a loading strain rate of 0.01 s 1 according to the ASTM D575 procedure , and at
an unloading rate of 1 mN/s. The surface of the compression platens was lubricated with Teﬂon spray. The applied load (F) on the specimen and the corresponding change in thickness (Δt) of the specimen were recorded. The planar surface area (Acomp ¼ 0.785 mm2, assumed to be constant), initial thickness (t0) and initial solidity (ϕ0) of the mat were used to convert the raw data from the UTM into mechanical stress (sm ¼F/Acomp), engineering strain (e¼Δt/t0) and solidity. ϕ¼
ϕ0 t 0 t 0 Δt
t0 was measured by the UTM with a contact force of 20 μN as described above. Eq. (1) was ﬁtted to the post-processed data of the unloading segment of the ﬁfth cycle in log–log form using unconstrained nonlinear optimization with the trust-region algorithm (fminunc in MATLAB v2011b), and the corresponding kE and n values were obtained. For further details, the reader is referred to the work of Choong et al.  on electrospun PSU mats evaluated in the dry state. 3.6. Permeance measurement The permeation test was carried out using a 25 mm diameter, polypropylene in-line ﬁlter holder (Sterlitech, PP25) as the dead-end ﬁltration cell. The electrospun mats were plasma treated at low power setting for 1 min, and then soaked in deionized (DI) water to ensure that the mats were wetted. The average of the permeance was calculated from three replicates. The permeance of water was measured for pressures ranging from 5 kPa to 140 kPa. The pressure was controlled by a pressurized air supply applied to the water on the feed side of the mat. Each mat was conditioned by ﬂowing water through at 140 kPa for 1 min before the permeation test. A permeation test consisted of measuring the permeance at successively higher pressures (from 5 kPa to 140 kPa) on the upstream side of the mat. 3.7. Permeance modeling The differential equations (Eqs. (5) and (6)) were solved numerically using backward differentiation formulae with orders 1–5 (ode15s in MATLAB v2011b) for solving stiff sets of equations. The inputs to the model were ﬁber diameter, mass and area of the membrane, thickness (t0), and the values for n and kE obtained
Fig. 2. SEM images of PSU mats with average, as-spun ﬁber diameters of (a) 0.8 μm and (b) 0.4 μm, annealed at different temperatures. (a.i) As-spun PSU with an average ﬁber diameter of 0.8 μm; (a.ii) PSU annealed at 190 1C with a post-treatment average ﬁber diameter of 0.8 μm; (a.iii) PSU annealed at 200 1C with a post-treatment average ﬁber diameter of 0.8 μm; (a.iv) PSU annealed at 210 1C with a post-treatment average ﬁber diameter of 0.9 μm. (b.i) As-spun PSU with an average ﬁber diameter of 0.4 μm and (b.ii) PSU annealed at 210 1C with a post-treatment average ﬁber diameter of 0.4 μm. The scale bars are 2 μm and 1 μm for the micrographs in (a) and (b), respectively.
L.T. (Simon) Choong et al. / Journal of Membrane Science 451 (2014) 111–116
from compression testing; the outputs were the permeance and the proﬁles for pressure and solidity through the thickness of the mat. Since the value of kE obtained from the compression test was judged to be imprecise , kE was then treated as the sole adjustable parameter to ﬁt the experimental permeance curve using a nonlinear equation solver with the Levenberg–Marquardt algorithm (fsolve in MATLAB v2011b).
4. Results and discussions
4.2. Compression Mechanical compression tests were performed on the annealed electrospun mats in the wet condition to obtain the compressibility parameters n and kE from Toll's model under conditions comparable to those present during permeation testing. The values of these two parameters increase with increasing annealing temperature, as reported in Table 1. This trend was also observed in compression tests performed on dry electrospun mats  but n values for the electrospun mats are consistently higher when wet. We speculate the increase in n values is due to the lubrication of ﬁber junctions when water is present, which results in more ﬁber slippage, hence higher n values .
4.1. Morphology 4.3. Permeance As-spun PSU mats with ﬁber diameter of (0.8 70.4) mm and (0.47 0.1) mm were successfully electrospun, as shown in Fig. 2. The average ﬁber diameter of the PSU mat annealed at 210 1C was slightly larger than that of the as-spun mat, as shown in Table 1. This could be due to ﬁbers welded together not only at the ﬁber– ﬁber contacts, but also along the ﬁber itself, at 210 1C. PSU mats with smaller ﬁber diameter (0.4 mm) have narrower ﬁber diameter distributions than those of PSU mats with larger ﬁber diameter (0.8 mm). The initial solidity (ϕ0), i.e. before any deformation, is independent of the annealing temperature of PSU mats but smaller for PSU with smaller ﬁber diameter.
Fig. 3a shows that permeance decreases with an increase in pressure drop for all of the electrospun PSU ﬁber mats. This is compelling evidence that the solidities of the electrospun mats increase as a result of compression under pressure driven ﬂow. The permeance of the PSU mat with smaller ﬁber diameter is smaller than that of the PSU mats with bigger ﬁber diameter over the range of pressure drops tested. This is in agreement with the ﬁber diameter dependence of Happel's permeability model, and is due to the higher speciﬁc area of contact between ﬁber and ﬂuid that is associated with smaller diameter ﬁbers.
Table 1 Compressibility properties of wet electrospun mats and the kE value obtained from the line of best ﬁt for permeance curves. The error bars reported from mechanical measurements were obtained from the standard deviation of ﬁve replicates. The standard deviations of the kE values are comparable to the orders of magnitude; these values should be interpreted with caution. The kE values reported from permeation tests are accurate to about 5%. Fiber diameter (μm)
Annealing temperature (1C)
Initial solidity, ϕ0
n (compression test)
(kE) (compression test) (MPa)
(kE) (permeation test using Happel's equation) (MPa)
(kE) (permeation test using Davies's equation) (MPa)
0.4 7 0.1 0.8 7 0.4 0.8 7 0.3 0.9 7 0.4
210 190 200 210
0.077 0.01 0.107 0.02 0.107 0.02 0.09 7 0.01
7.4 7 0.3 6.4 7 0.3 7.677 0.08 8.3 7 0.3
337 28 5707 180 8007 140 27007 1500
3700 85 730 1200
2000 45 550 1100
Fig. 3. (a) Experimentally measured permeances (symbols) and best ﬁts of model (i.e. minimal sum of least squares residuals, lines) plotted against pressure drop for the PSU mats with 0.8 μm ﬁber diameter annealed at 190 1C (circles, solid line), PSU with 0.8 μm ﬁber diameter annealed at 200 1C (squares, dot-dashed line), PSU with 0.9 μm ﬁber diameter annealed at 210 1C (diamonds, dashed line), and PSU with 0.4 μm ﬁber diameter annealed at 210 1C (crosses, dotted line); the values of n and kE used in the model are reported in Table 1. (b) The permeance from (a) converted to dimensionless permeability K/D2 vs. solidity and compared with Happel's equation for the dimensionless permeability K/D2 (from Eq. (4)). The symbols in (b) are the same as for (a); the solid line is Happel's model.
L.T. (Simon) Choong et al. / Journal of Membrane Science 451 (2014) 111–116
Ideally, it should be possible to predict the permeance of an electrospun mat using Toll's compressibility equation with n and kE measured independently by the compression test; however, as previously reported , there is a large uncertainty in the values of kE obtained experimentally, due to inhomogeneities both in the original mat and as well as variations in the response of each replicate to mechanical conditioning. Therefore, the kE value was treated here as the single adjustable parameter. By ﬁtting the kE value, the permeation model was able to predict the permeance in good agreement with the experimental permeance of all four sets of PSU mats (R2 40.94). The values of kE obtained by permeance testing for PSU mats with an average ﬁber diameter of 0.8 μm and 0.9 μm annealed at 200 1C and 210 1C, respectively, are similar to those obtained by compression testing; however, the kE values obtained by permeation and compression tests differ by at least an order of magnitude for the other two PSU mats. The kE values are tabulated in Table 1.
Fig. 4. Pressure (solid line) and solidity (dotted line) proﬁle along the z-axis of an electrospun PSU mat annealed at 210C, having an initial solidity of 0.09 and initial thickness of 136 μm. The pressure drop applied here was 140 kPa.
The data for permeance vs. pressure drop can be converted to dimensionless permeability (K/D2) vs. average solidity using Eqs. (2), (9) and (10). K D2
where Δz is the thickness of the electrospun mat estimated from the permeation model with the optimized kE value. The mat thickness was also used to calculate the average solidity of the mats at each pressure drop. ϕ¼
m ρAperm Δz
where m is the mass of the electrospun mat; ρ is the density of bulk PSU; and Aperm is the area of the electrospun mat used for the permeation test. According to Happel, K/D2 should be a function of solidity only. The data for the four mats collapse into a single curve, with a root mean squared deviation of 0.011 from Happel's model, after the effects of ﬁber diameter and compression of the mats are taken into account; this result is shown in Fig. 3b. This conﬁrms that Happel's model describes the experimental permeability well. Other models perform comparably . For example, repeating the analysis using Davies' empirical equation  in lieu of Happel's model results in optimal values for kE that are in only slightly poorer agreement with the values obtained directly by compression testing (cf. Table 1), and yields a root mean squared deviation in K/D2 vs. solidity of 0.015. Perhaps more importantly, this analysis conﬁrms that the compression predicted by the model using Toll's equation accurately describes the change in solidity with applied hydraulic pressure. Fig. 4 shows the proﬁles for hydraulic pressure (as a fraction of total pressure) and solidity through the thickness of the PSU mat with a ﬁber diameter of 0.9 μm, annealed at 210 1C. As seen from the same ﬁgure, the largest increase in solidity occurs near the upstream of the membrane (near z ¼0). This is because the sample has a high n value (n¼ 8.3); hence the term dϕ/dsm is large at small solidity, according to Eq. (6). However, the high n value ultimately results in a decrease in dϕ/dsm as the solidity increases. For purposes of comparison, permeation and compression tests were also performed on a commercial microﬁltration membrane, MF, with a nominal pore size of 3 μm. The MF membrane is not ﬁbrous in structure, and is believed to be made using a phase inversion process.
Fig. 5. (a) Experimental permeability constant (Eq. (9)) vs. pressure drop for PSU with 0.8 μm ﬁber diameter annealed at 190 1C (circles), PSU with 0.8 μm ﬁber diameter annealed at 200 1C (squares), PSU with 0.9 μm ﬁber diameter annealed at 210 1C (diamonds), PSU with 0.4 μm ﬁber diameter annealed at 210 1C (triangles), and microﬁltration membrane with 3 μm pore size (ﬁlled circles); (b) the stress vs. solidity plot for microﬁltration membrane with 3 μm pore size (squares) and PSU with 0.9 μm ﬁber diameter annealed at 210 1C (circles).
L.T. (Simon) Choong et al. / Journal of Membrane Science 451 (2014) 111–116
Fig. 5a shows the measured permeability constant for the MF membrane compared to those of the electrospun membranes. The permeability constant of the MF membrane was calculated using Eq. (9), without normalizing by D2. The change in thickness of the MF membrane was estimated from the stress vs. solidity plot obtained from the mechanical compression experiment, as shown in Fig. 5b. This estimated permeability of the MF membrane was an underestimation because the compressive stress (same as pressure drop) was assumed to be homogeneous throughout the membrane. The permeability of the MF membrane is higher than those of the PSU mats over the range of pressure from 8 kPa to 140 kPa tested in this work, even though the initial solidity of the electrospun mats is lower. This suggests that the electrospun mats may perform better at pressures below about 8 kPa, but perform less well at higher pressures due to the increase of solidity that comes with the higher compressibility of the PSU mats. The solidity of the PSU mats becomes higher than that of MF membrane at 1 kPa, as seen in Fig. 5b. The change in permeability of the MF membrane is about 37%, compared to 62–67% for the electrospun ﬁber mats over the pressure range of 5–140 kPa, consistent with its lower compressibility. 5. Conclusions The permeabilities of electrospun mats under pressure driven ﬂow are shown to be well described by a model for compressible ﬁbrous media that uses Darcy's law for pressure-driven ﬂow with Happel's model for permeability and Toll's model for compressibility. The solidity increases along the z-axis in the ﬂow direction, and the rate of increase of the solidity depends on the compressibility (parameterized by n and kE) of electrospun mats. The permeability test provides an alternative method to estimate the kE values of electrospun mats in addition to direct measurement via compression tests. Electrospun PSU mats perform well at low pressure (P o1 kPa), but this advantage of high porosity declines with increasing pressure due to their compressive nature. Acknowledgments The authors would like to thank Matthew Mannarino and Philip Reiser for the useful discussions and support in the permeation experiments. The funding of this project was provided by King Fahd University of Petroleum and Minerals (KFUPM) in Dhahran, Saudi Arabia, through the Center for Clean Water and Clean Energy at MIT and KFUPM under Project no. R5-CW-08. We would also like to acknowledge the Institute for Soldier Nanotechnology at MIT for use of facilities.
References  K. Yoon, B. Hsiao, B. Chu, Functional nanoﬁbers for environmental applications, Journal of Materials Chemistry 18 (2008) 5326–5334.  C. Burger, B. Hsiao, B. Chu, Nanoﬁbrous materials and their applications, Annual Review of Materials Science 36 (2006) 333–368.  L.T. Choong, M.M. Mannarino, S. Basu, G.C. Rutledge, Compressibility of electropsun ﬁber mats, Journal of Materials Science 48 (2013) 7827–7836.  N. Li, A. Fane, W. Ho, T. Matsuura, Advanced Membrane Technology and Applications, Wiley, New Jersey, 2008 (102 pp. (Fig. 5.1).  M.A. Biot, Consolidation settlement under a rectangular load distribution, Journal of Applied Physics 12 (1941) 426–430.  M.A. Biot, Theory of elasticity and consolidation for a porous anisotropic solid, Journal of Applied Physics 26 (1955) 182–185.  W.M. Lai, Van C. Mow, V. Roth, Effect of nonlinear strain-dependent permeability and rate of compression on the behavior of articular cartilage, Journal of Biomechanical Engineering 103 (1981) 61–66.  Van C. Mow, M.H. Holmes, W.M. Lai, Fluid transport and mechanical properties of articular cartilage: a review, Journal of Biomechanics 17 (5) (1984) 377–394.  S. Zhu, R.H. Pelton, K. Colliver, Mechanistic modeling of ﬂuid permeation through compressible ﬁber beds, Chemical Engineering Science 50 (22) (1995) 3557–3572.  M. Kataja, K. Hiltunen, J. Timonen, Flow of water and air in a compressible porous medium. A model of wet pressing of paper, Journal of Physics D: Applied Physics 25 (1992) 1053–1063.  K.A. Jönsson, B.T.L. Jönsson, Fluid ﬂow in compressible porous media: I: steady-state conditions, AIChE Journal 38 (9) (1992) 1340–1348.  K.A. Jönsson, B.T.L. Jönsson, Fluid ﬂow in compressible porous media: II: dynamic behavior, AIChE Journal 38 (9) (1992) 1349–1356.  J. Happel, Viscous ﬂow relative to arrays of cylinders, AIChE Journal 5 (1959) 174–177.  J.E. Drummond, M.I. Tahir, Laminar viscous ﬂow through regular arrays of parallel solid cylinders, International Journal of Multiphase Flow 10 (1984) 515–540.  S. Kuwabara, The forces experienced by randomly distributed parallel circular cylinders or spheres in a viscous ﬂow at small Reynolds number, Journal of Physical Society of Japan 14 (1959) 527–532.  L. Spielman, S.L. Goren, Model predicting pressure drop and ﬁltration efﬁciency in ﬁbrous media, Environmental Science and Technology 2 (1968) 279–287.  N. Mao, S.J. Russell, Directional permeability in homogeneous nonwoven structures Part I: the relationship between directional permeability and ﬁbre orientation, Journal of the Textile Institute 91 (2) (2000) 235–243.  N. Mao, S.J. Russell, Modeling permeability in homogeneous threedimensional nonwoven fabrics, Textile Research Journal 73 (11) (2003) 939–944.  C.N. Davies, Air Filtration, Academic, London, 1973.  D.S. Clague, R.J. Phillips, A numerical calculation of the hydraulic permeability of three-dimensional disordered ﬁbrous media, Physics of Fluids 9 (6) (1997) 1562–1572.  A. Tamayol, M. Bahrami, Transverse permeability of ﬁbrous porous media, Physical Review E 83 (2011) 046314.  G.W. Jackson, D.F. James, The permeability of ﬁbrous porous media, Canadian Society for Chemical Engineering 64 (1986) 364–374.  S. Toll, Packing mechanics of ﬁber reinforcements, Polymer Engineering and Science 38 (8) (1998) 1337–1350.  M.M. Mannarino, G.C. Rutledge, Mechanical and tribological properties of electrospun PA 6(3)T ﬁber mats, Polymer 56 (2012) 3017–3025.  ASTM Standard D575, 1991, Standard Test Methods for Rubber Properties in Compression, ASTM International, West Conshohocken, PA, 2012.